#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/14/4341481.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4341481
loop_
_publ_author_name
'Blankenship, Trevor V.'
'Wang, Xiaoping'
'Hoffmann, Christina'
'Latturner, Susan E.'
_publ_section_title
;
 LiCa3As2H and Ca14As6X7 (X = C, H, N): Two New Arsenide Hydride Phases
 Grown from Ca/Li Metal Flux.
;
_journal_issue                   19
_journal_name_full               'Inorganic chemistry'
_journal_page_first              10620
_journal_page_last               10626
_journal_paper_doi               10.1021/ic501722d
_journal_volume                  53
_journal_year                    2014
_chemical_formula_sum            'C0.445 H4.915 As6 Ca14 N1.135'
_chemical_formula_weight         1036.79
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           127
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   15.7027(2)
_cell_length_b                   15.7027(2)
_cell_length_c                   9.1043(2)
_cell_measurement_temperature    100(2)
_cell_volume                     2244.89(6)
_computing_cell_refinement       Mantid
_computing_data_collection       'SNS PyDas'
_computing_data_reduction        'Mantid and anvred2x'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.709
_diffrn_measured_fraction_theta_max 0.448
_diffrn_measurement_device_type  'TOPAZ 6-Li-glass area detectors at the SNS'
_diffrn_measurement_method       'TOF Laue'
_diffrn_radiation_source         'Spallation Neutron Source at ORNL, USA'
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     '0.5 - 3.5'
_diffrn_reflns_av_R_equivalents  0.0858
_diffrn_reflns_av_sigmaI/netI    0.0701
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            7364
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         36.31
_diffrn_reflns_theta_min         2.89
_exptl_absorpt_coefficient_mu    0.0700
_exptl_absorpt_correction_T_max  0.9722
_exptl_absorpt_correction_T_min  0.9255
_exptl_absorpt_correction_type   sphere
_exptl_absorpt_process_details
;
The linear absorption coefficient is wavelength dependent
and it is calculated as:
          mu = 0.333 + 0.367 * lambda  [cm⁻¹]
The value of 0.07000 (mm⁻¹)given in _exptl_absorpt_coefficient_mu
is the value at 1 Å
;
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    3.068
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             402
_exptl_crystal_size_max          1.20
_exptl_crystal_size_mid          0.70
_exptl_crystal_size_min          0.70
_refine_diff_density_max         1.021
_refine_diff_density_min         -1.082
_refine_diff_density_rms         0.185
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.180
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     88
_refine_ls_number_reflns         1330
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.180
_refine_ls_R_factor_all          0.0547
_refine_ls_R_factor_gt           0.0541
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0259P)²+8.0088P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0927
_refine_ls_wR_factor_ref         0.0930
_reflns_number_gt                1322
_reflns_number_total             1330
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            ic501722d_si_002.cif
_cod_data_source_block           Ca14As6X7neutron
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Tetragonal' changed to 'tetragonal'
according to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2827 2014-09-09 07:05:25Z andrius 
;
_cod_original_formula_sum        'Ca14 As6 C0.445 N1.135 H4.915'
_cod_database_code               4341481
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x+1/2, -y+1/2, -z'
'-x, -y, z'
'-x+1/2, y+1/2, -z'
'y+1/2, x+1/2, -z'
'y, -x, z'
'-y, x, z'
'-y+1/2, -x+1/2, -z'
'-x, -y, -z'
'-x-1/2, y-1/2, z'
'x, y, -z'
'x-1/2, -y-1/2, z'
'-y-1/2, -x-1/2, z'
'-y, x, -z'
'y, -x, -z'
'y-1/2, x-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
As1 As 0.28442(9) 0.21558(9) 0.0000 0.0043(4) Uani 1 4 d S
As2 As 0.23642(9) 0.26358(9) 0.5000 0.0040(4) Uani 1 4 d S
As3 As 0.19791(6) -0.00809(6) 0.24415(14) 0.00552(17) Uani 1 1 d .
Ca1 Ca 0.5000 0.0000 0.3198(3) 0.0037(4) Uani 1 4 d S
Ca2 Ca 0.34226(9) 0.15774(9) 0.3059(2) 0.0075(4) Uani 1 2 d S
Ca3 Ca 0.03125(13) 0.31289(13) 0.5000 0.0049(3) Uani 1 2 d S
Ca4 Ca 0.32161(13) 0.01933(13) 0.0000 0.0059(4) Uani 1 2 d S
Ca5 Ca 0.18338(9) 0.31662(9) -0.2100(2) 0.0074(4) Uani 1 2 d S
Ca6 Ca 0.0000 0.0000 0.2512(4) 0.0058(4) Uani 1 4 d S
Ca7 Ca 0.12112(15) 0.11365(15) 0.0000 0.0096(4) Uani 1 2 d S
Ca8 Ca 0.11875(15) 0.10891(15) 0.5000 0.0086(4) Uani 1 2 d S
X1N N 0.41616(6) 0.08384(6) 0.5000 0.0042(3) Uani 1 4 d S
X2C C 0.0000 0.0000 0.5000 0.0042(9) Uani 0.890(18) 8 d SP
X3N N 0.0000 0.0000 0.0000 0.0042(3) Uani 0.27(2) 8 d SP
X3H H 0.0000 0.0000 0.0000 0.06(2) Uani 0.43(2) 8 d SP
H1 H 0.3830(4) -0.1170(4) 0.0000 0.025(3) Uani 0.70(3) 4 d SP
H2 H 0.09923(16) 0.40077(16) -0.3388(4) 0.0204(6) Uani 1 2 d S
H3 H 0.42552(15) 0.07448(15) 0.1470(4) 0.0192(6) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ca5 As1 Ca5 80.88(10) 11 .
Ca5 As1 Ca7 80.12(5) 11 13_665
Ca5 As1 Ca7 80.12(5) . 13_665
Ca5 As1 Ca7 80.12(5) 11 .
Ca5 As1 Ca7 80.12(5) . .
Ca7 As1 Ca7 153.95(12) 13_665 .
Ca5 As1 Ca2 155.20(8) 11 11
Ca5 As1 Ca2 74.33(6) . 11
Ca7 As1 Ca2 95.42(2) 13_665 11
Ca7 As1 Ca2 95.42(2) . 11
Ca5 As1 Ca2 74.33(6) 11 .
Ca5 As1 Ca2 155.20(8) . .
Ca7 As1 Ca2 95.42(2) 13_665 .
Ca7 As1 Ca2 95.42(2) . .
Ca2 As1 Ca2 130.47(10) 11 .
Ca5 As1 Ca4 128.97(4) 11 13_665
Ca5 As1 Ca4 128.97(4) . 13_665
Ca7 As1 Ca4 68.76(6) 13_665 13_665
Ca7 As1 Ca4 137.30(8) . 13_665
Ca2 As1 Ca4 69.75(5) 11 13_665
Ca2 As1 Ca4 69.75(5) . 13_665
Ca5 As1 Ca4 128.97(4) 11 .
Ca5 As1 Ca4 128.97(4) . .
Ca7 As1 Ca4 137.30(8) 13_665 .
Ca7 As1 Ca4 68.76(6) . .
Ca2 As1 Ca4 69.75(5) 11 .
Ca2 As1 Ca4 69.75(5) . .
Ca4 As1 Ca4 68.54(8) 13_665 .
Ca5 As2 Ca5 131.91(11) 11 1_556
Ca5 As2 Ca2 77.10(6) 11 .
Ca5 As2 Ca2 150.99(8) 1_556 .
Ca5 As2 Ca2 150.99(8) 11 11_556
Ca5 As2 Ca2 77.10(6) 1_556 11_556
Ca2 As2 Ca2 73.89(10) . 11_556
Ca5 As2 Ca8 93.14(2) 11 13_665
Ca5 As2 Ca8 93.14(2) 1_556 13_665
Ca2 As2 Ca8 83.82(5) . 13_665
Ca2 As2 Ca8 83.82(5) 11_556 13_665
Ca5 As2 Ca8 93.14(2) 11 .
Ca5 As2 Ca8 93.14(2) 1_556 .
Ca2 As2 Ca8 83.82(5) . .
Ca2 As2 Ca8 83.82(5) 11_556 .
Ca8 As2 Ca8 164.53(11) 13_665 .
Ca5 As2 Ca3 69.67(5) 11 13_665
Ca5 As2 Ca3 69.67(5) 1_556 13_665
Ca2 As2 Ca3 132.97(4) . 13_665
Ca2 As2 Ca3 132.97(4) 11_556 13_665
Ca8 As2 Ca3 66.25(6) 13_665 13_665
Ca8 As2 Ca3 129.22(8) . 13_665
Ca5 As2 Ca3 69.67(5) 11 .
Ca5 As2 Ca3 69.67(5) 1_556 .
Ca2 As2 Ca3 132.97(4) . .
Ca2 As2 Ca3 132.97(4) 11_556 .
Ca8 As2 Ca3 129.22(8) 13_665 .
Ca8 As2 Ca3 66.25(6) . .
Ca3 As2 Ca3 62.97(8) 13_665 .
Ca3 As3 Ca4 101.90(5) 6 .
Ca3 As3 Ca6 126.60(8) 6 .
Ca4 As3 Ca6 131.29(8) . .
Ca3 As3 Ca7 137.98(7) 6 6
Ca4 As3 Ca7 80.12(5) . 6
Ca6 As3 Ca7 67.44(7) . 6
Ca3 As3 Ca7 148.77(7) 6 .
Ca4 As3 Ca7 68.78(6) . .
Ca6 As3 Ca7 67.04(7) . .
Ca7 As3 Ca7 71.58(7) 6 .
Ca3 As3 Ca8 74.74(6) 6 .
Ca4 As3 Ca8 135.13(6) . .
Ca6 As3 Ca8 64.89(7) . .
Ca7 As3 Ca8 132.32(6) 6 .
Ca7 As3 Ca8 90.94(5) . .
Ca3 As3 Ca8 68.34(5) 6 6
Ca4 As3 Ca8 153.93(6) . 6
Ca6 As3 Ca8 64.80(7) . 6
Ca7 As3 Ca8 91.38(5) 6 6
Ca7 As3 Ca8 131.81(6) . 6
Ca8 As3 Ca8 67.49(7) . 6
Ca3 As3 Ca5 68.44(6) 6 4_545
Ca4 As3 Ca5 71.71(6) . 4_545
Ca6 As3 Ca5 126.39(5) . 4_545
Ca7 As3 Ca5 72.73(6) 6 4_545
Ca7 As3 Ca5 130.11(6) . 4_545
Ca8 As3 Ca5 138.94(6) . 4_545
Ca8 As3 Ca5 82.24(6) 6 4_545
Ca3 As3 Ca2 64.60(6) 6 .
Ca4 As3 Ca2 65.81(5) . .
Ca6 As3 Ca2 127.85(5) . .
Ca7 As3 Ca2 143.93(6) 6 .
Ca7 As3 Ca2 84.84(6) . .
Ca8 As3 Ca2 73.08(6) . .
Ca8 As3 Ca2 124.47(6) 6 .
Ca5 As3 Ca2 105.48(5) 4_545 .
X1N Ca1 X1N 97.24(10) . 9_656
X1N Ca1 Ca1 48.62(5) . 9_656
X1N Ca1 Ca1 48.62(5) 9_656 9_656
X1N Ca1 Ca3 93.61(7) . 14_656
X1N Ca1 Ca3 45.51(4) 9_656 14_656
Ca1 Ca1 Ca3 61.16(4) 9_656 14_656
X1N Ca1 Ca3 45.51(4) . 2_556
X1N Ca1 Ca3 93.61(7) 9_656 2_556
Ca1 Ca1 Ca3 61.16(4) 9_656 2_556
Ca3 Ca1 Ca3 61.18(7) 14_656 2_556
X1N Ca1 Ca3 45.51(4) . 6
X1N Ca1 Ca3 93.61(7) 9_656 6
Ca1 Ca1 Ca3 61.16(4) 9_656 6
Ca3 Ca1 Ca3 122.32(9) 14_656 6
Ca3 Ca1 Ca3 90.95(8) 2_556 6
X1N Ca1 Ca3 93.61(7) . 10_655
X1N Ca1 Ca3 45.51(4) 9_656 10_655
Ca1 Ca1 Ca3 61.16(4) 9_656 10_655
Ca3 Ca1 Ca3 90.95(8) 14_656 10_655
Ca3 Ca1 Ca3 122.32(9) 2_556 10_655
Ca3 Ca1 Ca3 61.18(7) 6 10_655
X1N Ca1 Ca2 140.70(10) . 3_655
X1N Ca1 Ca2 43.46(4) 9_656 3_655
Ca1 Ca1 Ca2 92.08(6) 9_656 3_655
Ca3 Ca1 Ca2 60.59(4) 14_656 3_655
Ca3 Ca1 Ca2 121.74(5) 2_556 3_655
Ca3 Ca1 Ca2 121.74(5) 6 3_655
Ca3 Ca1 Ca2 60.59(4) 10_655 3_655
X1N Ca1 Ca2 43.46(4) . .
X1N Ca1 Ca2 140.70(10) 9_656 .
Ca1 Ca1 Ca2 92.08(6) 9_656 .
Ca3 Ca1 Ca2 121.74(5) 14_656 .
Ca3 Ca1 Ca2 60.59(4) 2_556 .
Ca3 Ca1 Ca2 60.59(4) 6 .
Ca3 Ca1 Ca2 121.74(5) 10_655 .
Ca2 Ca1 Ca2 175.84(12) 3_655 .
X1N Ca1 Ca4 93.93(3) . .
X1N Ca1 Ca4 151.84(3) 9_656 .
Ca1 Ca1 Ca4 135.94(3) 9_656 .
Ca3 Ca1 Ca4 158.93(6) 14_656 .
Ca3 Ca1 Ca4 112.44(4) 2_556 .
Ca3 Ca1 Ca4 76.12(3) 6 .
Ca3 Ca1 Ca4 108.16(4) 10_655 .
Ca2 Ca1 Ca4 121.02(7) 3_655 .
Ca2 Ca1 Ca4 55.42(4) . .
X1N Ca1 Ca4 151.84(3) . 5_545
X1N Ca1 Ca4 93.93(3) 9_656 5_545
Ca1 Ca1 Ca4 135.94(3) 9_656 5_545
Ca3 Ca1 Ca4 112.44(4) 14_656 5_545
Ca3 Ca1 Ca4 158.93(6) 2_556 5_545
Ca3 Ca1 Ca4 108.16(4) 6 5_545
Ca3 Ca1 Ca4 76.12(3) 10_655 5_545
Ca2 Ca1 Ca4 55.42(4) 3_655 5_545
Ca2 Ca1 Ca4 121.02(7) . 5_545
Ca4 Ca1 Ca4 65.62(6) . 5_545
X1N Ca1 Ca4 93.93(3) . 13_665
X1N Ca1 Ca4 151.84(3) 9_656 13_665
Ca1 Ca1 Ca4 135.94(3) 9_656 13_665
Ca3 Ca1 Ca4 108.16(4) 14_656 13_665
Ca3 Ca1 Ca4 76.12(3) 2_556 13_665
Ca3 Ca1 Ca4 112.44(4) 6 13_665
Ca3 Ca1 Ca4 158.93(6) 10_655 13_665
Ca2 Ca1 Ca4 121.02(7) 3_655 13_665
Ca2 Ca1 Ca4 55.42(4) . 13_665
Ca4 Ca1 Ca4 51.68(6) . 13_665
Ca4 Ca1 Ca4 88.12(7) 5_545 13_665
X1N Ca1 H3 84.94(9) . .
X1N Ca1 H3 177.82(13) 9_656 .
Ca1 Ca1 H3 133.56(10) 9_656 .
Ca3 Ca1 H3 134.52(4) 14_656 .
Ca3 Ca1 H3 87.92(7) 2_556 .
Ca3 Ca1 H3 87.92(7) 6 .
Ca3 Ca1 H3 134.52(4) 10_655 .
Ca2 Ca1 H3 134.36(13) 3_655 .
Ca2 Ca1 H3 41.48(10) . .
Ca4 Ca1 H3 27.39(4) . .
Ca4 Ca1 H3 84.11(11) 5_545 .
Ca4 Ca1 H3 27.39(4) 13_665 .
X1N Ca2 As2 95.93(8) . .
X1N Ca2 As1 161.89(10) . .
As2 Ca2 As1 102.18(7) . .
X1N Ca2 Ca3 44.13(4) . 2_556
As2 Ca2 Ca3 95.83(6) . 2_556
As1 Ca2 Ca3 132.35(4) . 2_556
X1N Ca2 Ca3 44.13(4) . 6
As2 Ca2 Ca3 95.83(6) . 6
As1 Ca2 Ca3 132.35(4) . 6
Ca3 Ca2 Ca3 88.17(7) 2_556 6
X1N Ca2 As3 94.09(4) . .
As2 Ca2 As3 98.69(4) . .
As1 Ca2 As3 83.27(4) . .
Ca3 Ca2 As3 137.04(7) 2_556 .
Ca3 Ca2 As3 50.34(3) 6 .
X1N Ca2 As3 94.09(4) . 13_665
As2 Ca2 As3 98.69(4) . 13_665
As1 Ca2 As3 83.27(4) . 13_665
Ca3 Ca2 As3 50.34(3) 2_556 13_665
Ca3 Ca2 As3 137.04(7) 6 13_665
As3 Ca2 As3 159.90(8) . 13_665
X1N Ca2 Ca1 45.04(6) . .
As2 Ca2 Ca1 140.97(9) . .
As1 Ca2 Ca1 116.85(9) . .
Ca3 Ca2 Ca1 58.22(5) 2_556 .
Ca3 Ca2 Ca1 58.22(5) 6 .
As3 Ca2 Ca1 86.43(4) . .
As3 Ca2 Ca1 86.43(4) 13_665 .
X1N Ca2 Ca2 42.87(6) . 11_556
As2 Ca2 Ca2 53.06(5) . 11_556
As1 Ca2 Ca2 155.24(5) . 11_556
Ca3 Ca2 Ca2 59.52(4) 2_556 11_556
Ca3 Ca2 Ca2 59.52(4) 6 11_556
As3 Ca2 Ca2 99.24(4) . 11_556
As3 Ca2 Ca2 99.24(4) 13_665 11_556
Ca1 Ca2 Ca2 87.92(6) . 11_556
X1N Ca2 Ca4 108.94(7) . .
As2 Ca2 Ca4 140.03(6) . .
As1 Ca2 Ca4 56.05(5) . .
Ca3 Ca2 Ca4 123.86(7) 2_556 .
Ca3 Ca2 Ca4 82.20(4) 6 .
As3 Ca2 Ca4 50.10(4) . .
As3 Ca2 Ca4 109.82(6) 13_665 .
Ca1 Ca2 Ca4 70.13(6) . .
Ca2 Ca2 Ca4 141.72(4) 11_556 .
X1N Ca2 Ca4 108.94(7) . 13_665
As2 Ca2 Ca4 140.03(6) . 13_665
As1 Ca2 Ca4 56.05(5) . 13_665
Ca3 Ca2 Ca4 82.20(4) 2_556 13_665
Ca3 Ca2 Ca4 123.86(7) 6 13_665
As3 Ca2 Ca4 109.82(6) . 13_665
As3 Ca2 Ca4 50.10(4) 13_665 13_665
Ca1 Ca2 Ca4 70.13(6) . 13_665
Ca2 Ca2 Ca4 141.72(4) 11_556 13_665
Ca4 Ca2 Ca4 59.72(7) . 13_665
X1N Ca2 Ca5 146.76(9) . 11
As2 Ca2 Ca5 50.83(5) . 11
As1 Ca2 Ca5 51.35(6) . 11
Ca3 Ca2 Ca5 127.99(5) 2_556 11
Ca3 Ca2 Ca5 127.98(5) 6 11
As3 Ca2 Ca5 91.58(4) . 11
As3 Ca2 Ca5 91.58(4) 13_665 11
Ca1 Ca2 Ca5 168.19(9) . 11
Ca2 Ca2 Ca5 103.89(5) 11_556 11
Ca4 Ca2 Ca5 99.75(6) . 11
Ca4 Ca2 Ca5 99.75(6) 13_665 11
X1N Ca2 H3 85.15(11) . .
As2 Ca2 H3 178.92(13) . .
As1 Ca2 H3 76.74(11) . .
Ca3 Ca2 H3 84.94(8) 2_556 .
Ca3 Ca2 H3 84.94(8) 6 .
As3 Ca2 H3 81.22(4) . .
As3 Ca2 H3 81.22(4) 13_665 .
Ca1 Ca2 H3 40.11(10) . .
Ca2 Ca2 H3 128.03(10) 11_556 .
Ca4 Ca2 H3 39.29(7) . .
Ca4 Ca2 H3 39.29(7) 13_665 .
Ca5 Ca2 H3 128.09(12) 11 .
X1N Ca3 As3 108.36(6) 2_456 7
X1N Ca3 As3 108.36(6) 2_456 14_556
As3 Ca3 As3 103.33(7) 7 14_556
X1N Ca3 As2 151.61(9) 2_456 .
As3 Ca3 As2 88.68(5) 7 .
As3 Ca3 As2 88.68(5) 14_556 .
X1N Ca3 Ca1 46.81(4) 2_456 2_456
As3 Ca3 Ca1 152.38(7) 7 2_456
As3 Ca3 Ca1 97.43(5) 14_556 2_456
As2 Ca3 Ca1 110.01(5) . 2_456
X1N Ca3 Ca1 46.81(4) 2_456 10_665
As3 Ca3 Ca1 97.43(5) 7 10_665
As3 Ca3 Ca1 152.38(7) 14_556 10_665
As2 Ca3 Ca1 110.01(5) . 10_665
Ca1 Ca3 Ca1 57.68(9) 2_456 10_665
X1N Ca3 Ca3 93.10(6) 2_456 13_665
As3 Ca3 Ca3 121.10(4) 7 13_665
As3 Ca3 Ca3 121.10(4) 14_556 13_665
As2 Ca3 Ca3 58.52(4) . 13_665
Ca1 Ca3 Ca3 59.41(4) 2_456 13_665
Ca1 Ca3 Ca3 59.41(4) 10_665 13_665
X1N Ca3 Ca2 43.76(4) 2_456 12_565
As3 Ca3 Ca2 65.06(4) 7 12_565
As3 Ca3 Ca2 111.97(7) 14_556 12_565
As2 Ca3 Ca2 149.20(4) . 12_565
Ca1 Ca3 Ca2 90.43(6) 2_456 12_565
Ca1 Ca3 Ca2 61.19(4) 10_665 12_565
Ca3 Ca3 Ca2 120.57(4) 13_665 12_565
X1N Ca3 Ca2 43.76(4) 2_456 2_456
As3 Ca3 Ca2 111.97(7) 7 2_456
As3 Ca3 Ca2 65.06(4) 14_556 2_456
As2 Ca3 Ca2 149.20(4) . 2_456
Ca1 Ca3 Ca2 61.19(4) 2_456 2_456
Ca1 Ca3 Ca2 90.43(6) 10_665 2_456
Ca3 Ca3 Ca2 120.57(4) 13_665 2_456
Ca2 Ca3 Ca2 60.96(7) 12_565 2_456
X1N Ca3 Ca8 155.12(10) 2_456 .
As3 Ca3 Ca8 59.30(4) 7 .
As3 Ca3 Ca8 59.30(4) 14_556 .
As2 Ca3 Ca8 53.27(5) . .
Ca1 Ca3 Ca8 148.31(5) 2_456 .
Ca1 Ca3 Ca8 148.31(5) 10_665 .
Ca3 Ca3 Ca8 111.78(5) 13_665 .
Ca2 Ca3 Ca8 117.22(6) 12_565 .
Ca2 Ca3 Ca8 117.22(6) 2_456 .
X1N Ca3 Ca5 119.23(6) 2_456 1_556
As3 Ca3 Ca5 132.35(8) 7 1_556
As3 Ca3 Ca5 60.70(3) 14_556 1_556
As2 Ca3 Ca5 49.57(4) . 1_556
Ca1 Ca3 Ca5 74.04(5) 2_456 1_556
Ca1 Ca3 Ca5 116.12(6) 10_665 1_556
Ca3 Ca3 Ca5 60.92(3) 13_665 1_556
Ca2 Ca3 Ca5 160.94(6) 12_565 1_556
Ca2 Ca3 Ca5 101.13(5) 2_456 1_556
Ca8 Ca3 Ca5 75.56(5) . 1_556
X1N Ca3 Ca5 119.23(6) 2_456 11
As3 Ca3 Ca5 60.70(3) 7 11
As3 Ca3 Ca5 132.35(8) 14_556 11
As2 Ca3 Ca5 49.57(4) . 11
Ca1 Ca3 Ca5 116.12(6) 2_456 11
Ca1 Ca3 Ca5 74.04(5) 10_665 11
Ca3 Ca3 Ca5 60.92(3) 13_665 11
Ca2 Ca3 Ca5 101.13(5) 12_565 11
Ca2 Ca3 Ca5 160.94(6) 2_456 11
Ca8 Ca3 Ca5 75.56(5) . 11
Ca5 Ca3 Ca5 95.70(8) 1_556 11
As3 Ca4 As3 96.34(7) 11 .
As3 Ca4 As1 91.18(5) 11 .
As3 Ca4 As1 91.18(5) . .
As3 Ca4 Ca7 58.15(4) 11 .
As3 Ca4 Ca7 58.15(4) . .
As1 Ca4 Ca7 54.07(5) . .
As3 Ca4 Ca4 124.23(4) 11 13_665
As3 Ca4 Ca4 124.23(4) . 13_665
As1 Ca4 Ca4 55.73(4) . 13_665
Ca7 Ca4 Ca4 109.81(5) . 13_665
As3 Ca4 Ca2 137.13(8) 11 .
As3 Ca4 Ca2 64.09(3) . .
As1 Ca4 Ca2 54.20(4) . .
Ca7 Ca4 Ca2 79.74(5) . .
Ca4 Ca4 Ca2 60.14(3) 13_665 .
As3 Ca4 Ca2 64.09(3) 11 11
As3 Ca4 Ca2 137.13(8) . 11
As1 Ca4 Ca2 54.20(4) . 11
Ca7 Ca4 Ca2 79.74(5) . 11
Ca4 Ca4 Ca2 60.14(3) 13_665 11
Ca2 Ca4 Ca2 103.44(7) . 11
As3 Ca4 Ca5 58.60(4) 11 10_655
As3 Ca4 Ca5 104.25(7) . 10_655
As1 Ca4 Ca5 146.94(4) . 10_655
Ca7 Ca4 Ca5 110.23(6) . 10_655
Ca4 Ca4 Ca5 128.38(4) 13_665 10_655
Ca2 Ca4 Ca5 158.62(6) . 10_655
Ca2 Ca4 Ca5 97.06(4) 11 10_655
As3 Ca4 Ca5 104.25(7) 11 4_545
As3 Ca4 Ca5 58.60(4) . 4_545
As1 Ca4 Ca5 146.94(4) . 4_545
Ca7 Ca4 Ca5 110.23(6) . 4_545
Ca4 Ca4 Ca5 128.38(4) 13_665 4_545
Ca2 Ca4 Ca5 97.06(4) . 4_545
Ca2 Ca4 Ca5 158.62(6) 11 4_545
Ca5 Ca4 Ca5 61.97(7) 10_655 4_545
As3 Ca4 Ca7 51.66(4) 11 6
As3 Ca4 Ca7 51.66(4) . 6
As1 Ca4 Ca7 113.30(7) . 6
Ca7 Ca4 Ca7 59.23(8) . 6
Ca4 Ca4 Ca7 169.04(5) 13_665 6
Ca2 Ca4 Ca7 114.75(4) . 6
Ca2 Ca4 Ca7 114.75(4) 11 6
Ca5 Ca4 Ca7 60.19(5) 10_655 6
Ca5 Ca4 Ca7 60.19(5) 4_545 6
As3 Ca4 Ca1 167.11(7) 11 .
As3 Ca4 Ca1 84.48(4) . .
As1 Ca4 Ca1 101.67(4) . .
Ca7 Ca4 Ca1 131.11(4) . .
Ca4 Ca4 Ca1 64.16(3) 13_665 .
Ca2 Ca4 Ca1 54.45(4) . .
Ca2 Ca4 Ca1 123.15(6) 11 .
Ca5 Ca4 Ca1 108.68(5) 10_655 .
Ca5 Ca4 Ca1 65.19(4) 4_545 .
Ca7 Ca4 Ca1 122.07(4) 6 .
As3 Ca4 Ca1 84.48(4) 11 9_655
As3 Ca4 Ca1 167.11(7) . 9_655
As1 Ca4 Ca1 101.67(4) . 9_655
Ca7 Ca4 Ca1 131.11(4) . 9_655
Ca4 Ca4 Ca1 64.16(3) 13_665 9_655
Ca2 Ca4 Ca1 123.15(6) . 9_655
Ca2 Ca4 Ca1 54.45(4) 11 9_655
Ca5 Ca4 Ca1 65.19(4) 10_655 9_655
Ca5 Ca4 Ca1 108.68(5) 4_545 9_655
Ca7 Ca4 Ca1 122.07(4) 6 9_655
Ca1 Ca4 Ca1 91.88(7) . 9_655
As3 Ca4 H1 97.80(14) 11 .
As3 Ca4 H1 97.80(14) . .
As1 Ca4 H1 166.5(2) . .
Ca7 Ca4 H1 139.4(2) . .
Ca4 Ca4 H1 110.76(19) 13_665 .
Ca2 Ca4 H1 121.41(9) . .
Ca2 Ca4 H1 121.41(9) 11 .
Ca5 Ca4 H1 39.40(11) 10_655 .
Ca5 Ca4 H1 39.40(11) 4_545 .
Ca7 Ca4 H1 80.2(2) 6 .
Ca1 Ca4 H1 69.38(13) . .
Ca1 Ca4 H1 69.38(13) 9_655 .
As3 Ca4 H3 163.29(10) 11 .
As3 Ca4 H3 94.77(8) . .
As1 Ca4 H3 76.13(10) . .
Ca7 Ca4 H3 119.05(11) . .
Ca4 Ca4 H3 39.27(8) 13_665 .
Ca2 Ca4 H3 40.65(10) . .
Ca2 Ca4 H3 99.36(9) 11 .
Ca5 Ca4 H3 129.98(12) 10_655 .
Ca5 Ca4 H3 92.19(8) 4_545 .
Ca7 Ca4 H3 143.63(8) 6 .
Ca1 Ca4 H3 27.41(7) . .
Ca1 Ca4 H3 87.46(11) 9_655 .
H1 Ca4 H3 93.01(18) . .
As2 Ca5 As1 106.39(8) 1_554 .
As2 Ca5 As3 89.52(4) 1_554 4
As1 Ca5 As3 101.74(4) . 4
As2 Ca5 As3 89.52(4) 1_554 14
As1 Ca5 As3 101.74(4) . 14
As3 Ca5 As3 155.77(8) 4 14
As2 Ca5 Ca3 60.76(5) 1_554 1_554
As1 Ca5 Ca3 146.42(5) . 1_554
As3 Ca5 Ca3 108.61(6) 4 1_554
As3 Ca5 Ca3 50.86(4) 14 1_554
As2 Ca5 Ca3 60.76(5) 1_554 13_664
As1 Ca5 Ca3 146.42(5) . 13_664
As3 Ca5 Ca3 50.86(4) 4 13_664
As3 Ca5 Ca3 108.61(6) 14 13_664
Ca3 Ca5 Ca3 58.16(7) 1_554 13_664
As2 Ca5 Ca2 52.07(6) 1_554 11
As1 Ca5 Ca2 54.33(5) . 11
As3 Ca5 Ca2 99.23(4) 4 11
As3 Ca5 Ca2 99.23(4) 14 11
Ca3 Ca5 Ca2 105.74(7) 1_554 11
Ca3 Ca5 Ca2 105.74(7) 13_664 11
As2 Ca5 Ca4 136.32(5) 1_554 10_665
As1 Ca5 Ca4 97.97(6) . 10_665
As3 Ca5 Ca4 49.70(4) 4 10_665
As3 Ca5 Ca4 120.60(7) 14 10_665
Ca3 Ca5 Ca4 112.43(7) 1_554 10_665
Ca3 Ca5 Ca4 78.88(4) 13_664 10_665
Ca2 Ca5 Ca4 136.58(5) 11 10_665
As2 Ca5 Ca4 136.32(5) 1_554 14
As1 Ca5 Ca4 97.97(6) . 14
As3 Ca5 Ca4 120.60(7) 4 14
As3 Ca5 Ca4 49.70(4) 14 14
Ca3 Ca5 Ca4 78.88(4) 1_554 14
Ca3 Ca5 Ca4 112.43(7) 13_664 14
Ca2 Ca5 Ca4 136.58(5) 11 14
Ca4 Ca5 Ca4 72.47(7) 10_665 14
As2 Ca5 Ca5 155.95(5) 1_554 11
As1 Ca5 Ca5 49.56(5) . 11
As3 Ca5 Ca5 95.34(4) 4 11
As3 Ca5 Ca5 95.34(4) 14 11
Ca3 Ca5 Ca5 137.85(4) 1_554 11
Ca3 Ca5 Ca5 137.85(4) 13_664 11
Ca2 Ca5 Ca5 103.89(5) 11 11
Ca4 Ca5 Ca5 59.01(4) 10_665 11
Ca4 Ca5 Ca5 59.01(4) 14 11
As2 Ca5 Ca7 106.78(5) 1_554 13_665
As1 Ca5 Ca7 50.79(4) . 13_665
As3 Ca5 Ca7 51.21(4) 4 13_665
As3 Ca5 Ca7 150.69(7) 14 13_665
Ca3 Ca5 Ca7 158.34(6) 1_554 13_665
Ca3 Ca5 Ca7 100.64(4) 13_664 13_665
Ca2 Ca5 Ca7 74.02(5) 11 13_665
Ca4 Ca5 Ca7 62.83(5) 10_665 13_665
Ca4 Ca5 Ca7 116.69(6) 14 13_665
Ca5 Ca5 Ca7 60.16(3) 11 13_665
As2 Ca5 Ca7 106.78(5) 1_554 .
As1 Ca5 Ca7 50.79(4) . .
As3 Ca5 Ca7 150.69(7) 4 .
As3 Ca5 Ca7 51.21(4) 14 .
Ca3 Ca5 Ca7 100.64(4) 1_554 .
Ca3 Ca5 Ca7 158.34(6) 13_664 .
Ca2 Ca5 Ca7 74.02(5) 11 .
Ca4 Ca5 Ca7 116.69(6) 10_665 .
Ca4 Ca5 Ca7 62.83(5) 14 .
Ca5 Ca5 Ca7 60.16(3) 11 .
Ca7 Ca5 Ca7 100.04(8) 13_665 .
As2 Ca5 H2 81.95(12) 1_554 .
As1 Ca5 H2 171.65(14) . .
As3 Ca5 H2 77.95(4) 4 .
As3 Ca5 H2 77.95(4) 14 .
Ca3 Ca5 H2 38.19(7) 1_554 .
Ca3 Ca5 H2 38.19(7) 13_664 .
Ca2 Ca5 H2 134.02(13) 11 .
Ca4 Ca5 H2 75.37(9) 10_665 .
Ca4 Ca5 H2 75.37(9) 14 .
Ca5 Ca5 H2 122.09(11) 11 .
Ca7 Ca5 H2 127.50(5) 13_665 .
Ca7 Ca5 H2 127.50(5) . .
X2C Ca6 X3N 180.0 . .
X2C Ca6 As3 91.18(7) . 7
X3N Ca6 As3 88.82(7) . 7
X2C Ca6 As3 91.18(7) . .
X3N Ca6 As3 88.82(7) . .
As3 Ca6 As3 89.976(3) 7 .
X2C Ca6 As3 91.18(7) . 6
X3N Ca6 As3 88.82(7) . 6
As3 Ca6 As3 177.64(14) 7 6
As3 Ca6 As3 89.976(3) . 6
X2C Ca6 As3 91.18(7) . 3
X3N Ca6 As3 88.82(7) . 3
As3 Ca6 As3 89.976(3) 7 3
As3 Ca6 As3 177.64(14) . 3
As3 Ca6 As3 89.976(3) 6 3
X2C Ca6 Ca8 48.16(5) . .
X3N Ca6 Ca8 131.84(5) . .
As3 Ca6 Ca8 59.22(5) 7 .
As3 Ca6 Ca8 59.06(5) . .
As3 Ca6 Ca8 122.63(9) 6 .
As3 Ca6 Ca8 122.80(9) 3 .
X2C Ca6 Ca8 48.16(5) . 14_556
X3N Ca6 Ca8 131.84(5) . 14_556
As3 Ca6 Ca8 59.06(5) 7 14_556
As3 Ca6 Ca8 122.63(9) . 14_556
As3 Ca6 Ca8 122.80(9) 6 14_556
As3 Ca6 Ca8 59.22(5) 3 14_556
Ca8 Ca6 Ca8 63.58(6) . 14_556
X2C Ca6 Ca8 48.16(5) . 6
X3N Ca6 Ca8 131.84(5) . 6
As3 Ca6 Ca8 122.80(9) 7 6
As3 Ca6 Ca8 59.22(5) . 6
As3 Ca6 Ca8 59.06(5) 6 6
As3 Ca6 Ca8 122.63(9) 3 6
Ca8 Ca6 Ca8 63.58(6) . 6
Ca8 Ca6 Ca8 96.33(10) 14_556 6
X2C Ca6 Ca8 48.16(5) . 9_556
X3N Ca6 Ca8 131.84(5) . 9_556
As3 Ca6 Ca8 122.63(9) 7 9_556
As3 Ca6 Ca8 122.80(9) . 9_556
As3 Ca6 Ca8 59.22(5) 6 9_556
As3 Ca6 Ca8 59.06(5) 3 9_556
Ca8 Ca6 Ca8 96.33(10) . 9_556
Ca8 Ca6 Ca8 63.58(6) 14_556 9_556
Ca8 Ca6 Ca8 63.58(6) 6 9_556
X2C Ca6 Ca7 131.25(5) . 9
X3N Ca6 Ca7 48.75(5) . 9
As3 Ca6 Ca7 121.52(9) 7 9
As3 Ca6 Ca7 120.87(9) . 9
As3 Ca6 Ca7 56.64(5) 6 9
As3 Ca6 Ca7 57.30(5) 3 9
Ca8 Ca6 Ca7 179.23(9) . 9
Ca8 Ca6 Ca7 116.50(5) 14_556 9
Ca8 Ca6 Ca7 115.68(5) 6 9
Ca8 Ca6 Ca7 83.08(3) 9_556 9
X2C Ca6 Ca7 131.25(5) . 6
X3N Ca6 Ca7 48.75(5) . 6
As3 Ca6 Ca7 120.87(9) 7 6
As3 Ca6 Ca7 56.64(5) . 6
As3 Ca6 Ca7 57.30(5) 6 6
As3 Ca6 Ca7 121.52(9) 3 6
Ca8 Ca6 Ca7 115.68(5) . 6
Ca8 Ca6 Ca7 179.23(9) 14_556 6
Ca8 Ca6 Ca7 83.08(3) 6 6
Ca8 Ca6 Ca7 116.50(5) 9_556 6
Ca7 Ca6 Ca7 64.24(6) 9 6
X2C Ca6 X3H 180.0 . .
X3N Ca6 X3H 0.0 . .
As3 Ca6 X3H 88.82(7) 7 .
As3 Ca6 X3H 88.82(7) . .
As3 Ca6 X3H 88.82(7) 6 .
As3 Ca6 X3H 88.82(7) 3 .
Ca8 Ca6 X3H 131.84(5) . .
Ca8 Ca6 X3H 131.84(5) 14_556 .
Ca8 Ca6 X3H 131.84(5) 6 .
Ca8 Ca6 X3H 131.84(5) 9_556 .
Ca7 Ca6 X3H 48.75(5) 9 .
Ca7 Ca6 X3H 48.75(5) 6 .
X3N Ca7 As1 168.80(10) . .
X3N Ca7 As3 82.88(6) . 14
As1 Ca7 As3 104.87(6) . 14
X3N Ca7 As3 82.88(6) . 7
As1 Ca7 As3 104.87(6) . 7
As3 Ca7 As3 90.23(7) 14 7
X3N Ca7 As3 82.23(6) . 11
As1 Ca7 As3 89.81(6) . 11
As3 Ca7 As3 88.44(4) 14 11
As3 Ca7 As3 165.09(9) 7 11
X3N Ca7 As3 82.23(6) . .
As1 Ca7 As3 89.81(6) . .
As3 Ca7 As3 165.09(9) 14 .
As3 Ca7 As3 88.44(4) 7 .
As3 Ca7 As3 89.04(7) 11 .
X3N Ca7 Ca6 41.25(5) . 9
As1 Ca7 Ca6 137.52(5) . 9
As3 Ca7 Ca6 55.92(4) 14 9
As3 Ca7 Ca6 111.96(8) 7 9
As3 Ca7 Ca6 55.67(4) 11 9
As3 Ca7 Ca6 111.13(8) . 9
X3N Ca7 Ca6 41.25(5) . .
As1 Ca7 Ca6 137.52(5) . .
As3 Ca7 Ca6 111.96(8) 14 .
As3 Ca7 Ca6 55.92(4) 7 .
As3 Ca7 Ca6 111.13(8) 11 .
As3 Ca7 Ca6 55.67(4) . .
Ca6 Ca7 Ca6 82.49(10) 9 .
X3N Ca7 Ca4 111.63(8) . .
As1 Ca7 Ca4 57.17(7) . .
As3 Ca7 Ca4 133.75(4) 14 .
As3 Ca7 Ca4 133.75(4) 7 .
As3 Ca7 Ca4 53.07(4) 11 .
As3 Ca7 Ca4 53.07(4) . .
Ca6 Ca7 Ca4 106.09(6) 9 .
Ca6 Ca7 Ca4 106.09(6) . .
X3N Ca7 Ca7 45.0 . 6
As1 Ca7 Ca7 123.80(10) . 6
As3 Ca7 Ca7 113.80(4) 14 6
As3 Ca7 Ca7 113.80(4) 7 6
As3 Ca7 Ca7 53.80(6) 11 6
As3 Ca7 Ca7 53.80(6) . 6
Ca6 Ca7 Ca7 57.88(3) 9 6
Ca6 Ca7 Ca7 57.88(3) . 6
Ca4 Ca7 Ca7 66.63(8) . 6
X3N Ca7 Ca7 45.0 . 14
As1 Ca7 Ca7 146.20(10) . 14
As3 Ca7 Ca7 54.63(6) 14 14
As3 Ca7 Ca7 54.63(6) 7 14
As3 Ca7 Ca7 113.54(4) 11 14
As3 Ca7 Ca7 113.54(4) . 14
Ca6 Ca7 Ca7 57.88(3) 9 14
Ca6 Ca7 Ca7 57.88(3) . 14
Ca4 Ca7 Ca7 156.63(8) . 14
Ca7 Ca7 Ca7 90.0 6 14
X3N Ca7 Ca5 138.85(6) . 11
As1 Ca7 Ca5 49.09(5) . 11
As3 Ca7 Ca5 98.44(7) 14 11
As3 Ca7 Ca5 56.06(4) 7 11
As3 Ca7 Ca5 138.79(8) 11 11
As3 Ca7 Ca5 93.12(5) . 11
Ca6 Ca7 Ca5 153.40(8) 9 11
Ca6 Ca7 Ca5 103.77(5) . 11
Ca4 Ca7 Ca5 97.06(7) . 11
Ca7 Ca7 Ca5 146.82(6) 6 11
Ca7 Ca7 Ca5 103.17(8) 14 11
X3N Ca7 X3H 0.0 . .
As1 Ca7 X3H 168.80(10) . .
As3 Ca7 X3H 82.88(6) 14 .
As3 Ca7 X3H 82.88(6) 7 .
As3 Ca7 X3H 82.23(6) 11 .
As3 Ca7 X3H 82.23(6) . .
Ca6 Ca7 X3H 41.25(5) 9 .
Ca6 Ca7 X3H 41.25(5) . .
Ca4 Ca7 X3H 111.63(8) . .
Ca7 Ca7 X3H 45.0 6 .
Ca7 Ca7 X3H 45.0 14 .
Ca5 Ca7 X3H 138.85(6) 11 .
X2C Ca8 As2 169.79(10) . .
X2C Ca8 As3 84.19(5) . .
As2 Ca8 As3 102.74(6) . .
X2C Ca8 As3 84.19(5) . 11_556
As2 Ca8 As3 102.74(6) . 11_556
As3 Ca8 As3 92.80(7) . 11_556
X2C Ca8 As3 84.02(6) . 7
As2 Ca8 As3 88.93(6) . 7
As3 Ca8 As3 86.14(4) . 7
As3 Ca8 As3 168.21(8) 11_556 7
X2C Ca8 As3 84.02(6) . 14_556
As2 Ca8 As3 88.93(6) . 14_556
As3 Ca8 As3 168.21(8) . 14_556
As3 Ca8 As3 86.14(4) 11_556 14_556
As3 Ca8 As3 92.50(7) 7 14_556
X2C Ca8 Ca6 41.84(5) . .
As2 Ca8 Ca6 137.16(5) . .
As3 Ca8 Ca6 56.05(4) . .
As3 Ca8 Ca6 114.05(8) 11_556 .
As3 Ca8 Ca6 55.98(4) 7 .
As3 Ca8 Ca6 113.84(7) 14_556 .
X2C Ca8 Ca6 41.84(5) . 9_556
As2 Ca8 Ca6 137.16(5) . 9_556
As3 Ca8 Ca6 114.05(8) . 9_556
As3 Ca8 Ca6 56.05(4) 11_556 9_556
As3 Ca8 Ca6 113.84(7) 7 9_556
As3 Ca8 Ca6 55.98(4) 14_556 9_556
Ca6 Ca8 Ca6 83.67(10) . 9_556
X2C Ca8 Ca3 109.31(8) . .
As2 Ca8 Ca3 60.48(6) . .
As3 Ca8 Ca3 132.63(4) . .
As3 Ca8 Ca3 132.63(4) 11_556 .
As3 Ca8 Ca3 52.36(4) 7 .
As3 Ca8 Ca3 52.36(4) 14_556 .
Ca6 Ca8 Ca3 104.26(6) . .
Ca6 Ca8 Ca3 104.26(6) 9_556 .
X2C Ca8 Ca8 45.0 . 14_556
As2 Ca8 Ca8 124.79(10) . 14_556
As3 Ca8 Ca8 114.25(4) . 14_556
As3 Ca8 Ca8 114.25(4) 11_556 14_556
As3 Ca8 Ca8 56.15(6) 7 14_556
As3 Ca8 Ca8 56.15(6) 14_556 14_556
Ca6 Ca8 Ca8 58.21(3) . 14_556
Ca6 Ca8 Ca8 58.21(3) 9_556 14_556
Ca3 Ca8 Ca8 64.31(8) . 14_556
X2C Ca8 Ca8 45.0 . 6
As2 Ca8 Ca8 145.21(10) . 6
As3 Ca8 Ca8 56.36(6) . 6
As3 Ca8 Ca8 56.36(6) 11_556 6
As3 Ca8 Ca8 114.19(4) 7 6
As3 Ca8 Ca8 114.19(4) 14_556 6
Ca6 Ca8 Ca8 58.21(3) . 6
Ca6 Ca8 Ca8 58.21(3) 9_556 6
Ca3 Ca8 Ca8 154.31(8) . 6
Ca8 Ca8 Ca8 90.0 14_556 6
X2C Ca8 Ca3 101.65(7) . 6
As2 Ca8 Ca3 88.56(7) . 6
As3 Ca8 Ca3 49.64(4) . 6
As3 Ca8 Ca3 49.64(4) 11_556 6
As3 Ca8 Ca3 133.68(4) 7 6
As3 Ca8 Ca3 133.68(4) 14_556 6
Ca6 Ca8 Ca3 98.65(5) . 6
Ca6 Ca8 Ca3 98.65(5) 9_556 6
Ca3 Ca8 Ca3 149.05(8) . 6
Ca8 Ca8 Ca3 146.65(7) 14_556 6
Ca8 Ca8 Ca3 56.65(7) 6 6
Ca2 X1N Ca2 94.25(11) . 11_556
Ca2 X1N Ca3 92.11(4) . 2_556
Ca2 X1N Ca3 92.11(4) 11_556 2_556
Ca2 X1N Ca3 92.11(4) . 6
Ca2 X1N Ca3 92.11(4) 11_556 6
Ca3 X1N Ca3 173.81(12) 2_556 6
Ca2 X1N Ca1 91.49(7) . .
Ca2 X1N Ca1 174.26(8) 11_556 .
Ca3 X1N Ca1 87.68(4) 2_556 .
Ca3 X1N Ca1 87.68(4) 6 .
Ca2 X1N Ca1 174.26(8) . 9_656
Ca2 X1N Ca1 91.49(7) 11_556 9_656
Ca3 X1N Ca1 87.68(4) 2_556 9_656
Ca3 X1N Ca1 87.68(4) 6 9_656
Ca1 X1N Ca1 82.76(10) . 9_656
Ca6 X2C Ca6 180.0 . 9_556
Ca6 X2C Ca8 90.0 . 14_556
Ca6 X2C Ca8 90.0 9_556 14_556
Ca6 X2C Ca8 90.0 . .
Ca6 X2C Ca8 90.0 9_556 .
Ca8 X2C Ca8 90.0 14_556 .
Ca6 X2C Ca8 90.0 . 9_556
Ca6 X2C Ca8 90.0 9_556 9_556
Ca8 X2C Ca8 90.0 14_556 9_556
Ca8 X2C Ca8 180.00(10) . 9_556
Ca6 X2C Ca8 90.0 . 6
Ca6 X2C Ca8 90.0 9_556 6
Ca8 X2C Ca8 180.0 14_556 6
Ca8 X2C Ca8 90.0 . 6
Ca8 X2C Ca8 90.0 9_556 6
Ca6 X3N Ca6 180.0 9 .
Ca6 X3N Ca7 90.0 9 9
Ca6 X3N Ca7 90.0 . 9
Ca6 X3N Ca7 90.0 9 .
Ca6 X3N Ca7 90.0 . .
Ca7 X3N Ca7 180.00(11) 9 .
Ca6 X3N Ca7 90.0 9 14
Ca6 X3N Ca7 90.0 . 14
Ca7 X3N Ca7 90.0 9 14
Ca7 X3N Ca7 90.0 . 14
Ca6 X3N Ca7 90.0 9 6
Ca6 X3N Ca7 90.0 . 6
Ca7 X3N Ca7 90.0 9 6
Ca7 X3N Ca7 90.0 . 6
Ca7 X3N Ca7 180.00(11) 14 6
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
As1 Ca5 2.948(3) 11
As1 Ca5 2.948(3) .
As1 Ca7 3.023(2) 13_665
As1 Ca7 3.023(2) .
As1 Ca2 3.067(2) 11
As1 Ca2 3.067(2) .
As1 Ca4 3.136(3) 13_665
As1 Ca4 3.136(3) .
As2 Ca5 2.891(2) 11
As2 Ca5 2.891(2) 1_556
As2 Ca2 2.941(3) .
As2 Ca2 2.941(3) 11_556
As2 Ca8 3.052(2) 13_665
As2 Ca8 3.052(2) .
As2 Ca3 3.314(3) 13_665
As2 Ca3 3.314(3) .
As3 Ca3 2.9695(17) 6
As3 Ca4 2.9832(18) .
As3 Ca6 3.1110(9) .
As3 Ca7 3.137(2) 6
As3 Ca7 3.170(2) .
As3 Ca8 3.217(2) .
As3 Ca8 3.225(2) 6
As3 Ca5 3.3388(10) 4_545
As3 Ca2 3.4978(10) .
Ca1 X1N 2.481(2) .
Ca1 X1N 2.481(2) 9_656
Ca1 Ca1 3.281(6) 9_656
Ca1 Ca3 3.401(2) 14_656
Ca1 Ca3 3.401(2) 2_556
Ca1 Ca3 3.401(2) 6
Ca1 Ca3 3.401(2) 10_655
Ca1 Ca2 3.505(2) 3_655
Ca1 Ca2 3.505(2) .
Ca1 Ca4 4.052(2) .
Ca1 Ca4 4.052(2) 5_545
Ca1 Ca4 4.052(2) 13_665
Ca1 H3 2.283(4) .
Ca2 X1N 2.412(2) .
Ca2 Ca3 3.485(2) 2_556
Ca2 Ca3 3.485(2) 6
Ca2 As3 3.4978(10) 13_665
Ca2 Ca2 3.535(4) 11_556
Ca2 Ca4 3.547(2) .
Ca2 Ca4 3.547(2) 13_665
Ca2 Ca5 3.635(3) 11
Ca2 H3 2.347(4) .
Ca3 X1N 2.428(2) 2_456
Ca3 As3 2.9695(17) 7
Ca3 As3 2.9695(17) 14_556
Ca3 Ca1 3.401(2) 2_456
Ca3 Ca1 3.401(2) 10_665
Ca3 Ca3 3.461(4) 13_665
Ca3 Ca2 3.485(2) 12_565
Ca3 Ca2 3.485(2) 2_456
Ca3 Ca8 3.485(3) .
Ca3 Ca5 3.561(2) 1_556
Ca3 Ca5 3.561(2) 11
Ca4 As3 2.9832(18) 11
Ca4 Ca7 3.479(3) .
Ca4 Ca4 3.532(4) 13_665
Ca4 Ca2 3.547(2) 11
Ca4 Ca5 3.714(2) 10_655
Ca4 Ca5 3.714(2) 4_545
Ca4 Ca7 3.941(3) 6
Ca4 Ca1 4.052(2) 9_655
Ca4 H1 2.348(4) .
Ca4 H3 2.281(3) .
Ca5 As2 2.891(2) 1_554
Ca5 As3 3.3388(10) 4
Ca5 As3 3.3388(10) 14
Ca5 Ca3 3.561(2) 1_554
Ca5 Ca3 3.561(2) 13_664
Ca5 Ca2 3.635(3) 11
Ca5 Ca4 3.714(2) 10_665
Ca5 Ca4 3.714(2) 14
Ca5 Ca5 3.824(4) 11
Ca5 Ca7 3.843(2) 13_665
Ca5 Ca7 3.843(2) .
Ca5 H2 2.206(4) .
Ca6 X2C 2.265(4) .
Ca6 X3N 2.287(4) .
Ca6 As3 3.1110(9) 7
Ca6 As3 3.1110(9) 6
Ca6 As3 3.1110(9) 3
Ca6 Ca8 3.396(3) .
Ca6 Ca8 3.396(3) 14_556
Ca6 Ca8 3.396(3) 6
Ca6 Ca8 3.396(3) 9_556
Ca6 Ca7 3.469(3) 9
Ca6 Ca7 3.469(3) 6
Ca6 X3H 2.287(4) .
Ca7 X3N 2.608(2) .
Ca7 As3 3.137(2) 14
Ca7 As3 3.137(2) 7
Ca7 As3 3.170(2) 11
Ca7 Ca6 3.469(3) 9
Ca7 Ca7 3.688(3) 6
Ca7 Ca7 3.688(3) 14
Ca7 Ca5 3.843(2) 11
Ca7 X3H 2.608(2) .
Ca8 X2C 2.530(2) .
Ca8 As3 3.217(2) 11_556
Ca8 As3 3.225(2) 7
Ca8 As3 3.225(2) 14_556
Ca8 Ca6 3.396(3) 9_556
Ca8 Ca8 3.578(3) 14_556
Ca8 Ca8 3.578(3) 6
Ca8 Ca3 3.760(3) 6
X1N Ca2 2.412(2) 11_556
X1N Ca3 2.428(2) 2_556
X1N Ca3 2.428(2) 6
X1N Ca1 2.481(2) 9_656
X2C Ca6 2.265(4) 9_556
X2C Ca8 2.530(2) 14_556
X2C Ca8 2.530(2) 9_556
X2C Ca8 2.530(2) 6
X3N Ca6 2.287(4) 9
X3N Ca7 2.608(2) 9
X3N Ca7 2.608(2) 14
X3N Ca7 2.608(2) 6
X3N X3H 0.0000 .
